synthesis of organic/inorganic hybrid quatrefoil-shaped star-cyclic polymer containing a polyhedral...
Post on 27-Jan-2017
Embed Size (px)
Synthesis of Organic/Inorganic Hybrid Quatrefoil-Shaped Star-CyclicPolymer Containing a Polyhedral Oligomeric Silsesquioxane Core
Zhishen Ge, Di Wang, Yueming Zhou, Hewen Liu, and Shiyong Liu*
CAS Key Laboratory of Soft Matter Chemistry, Department of Polymer Science and Engineering, HefeiNational Laboratory for Physical Sciences at the Microscale, UniVersity of Science and Technology ofChina, Hefei, Anhui 230026, China
ReceiVed NoVember 22, 2008; ReVised Manuscript ReceiVed March 9, 2009
ABSTRACT: We report the synthesis of quatrefoil-shaped star-cyclic polystyrene, star-cyclic PS, containing apolyhedral oligomeric silsesquioxane (POSS) core via the combination of atom transfer radical polymerization(ATRP) and click chemistry techniques. The obtained star-cyclic PS represents a new chain topology in thecategory of nonlinear-shaped polymers. Using octa(3-chloropropyl) polyhedral oligomeric silsesquioxane, POSS-(Cl)8, as the starting material, its azidation and subsequent click reaction with a slight excess of propargyl2-bromobutyrate afforded octafunctional initiator, POSS-(Br)8. 8-arm star-linear PS-N3 was obtained by theazidation of star-linear PS-Br, which was synthesized by the ATRP of styrene using POSS-(Br)8 as the initiator.Model reaction between R,-diazido-terminated PS (N3-PS-N3) and difunctional propargyl ether confirmed thatbimolecular click cyclization reaction can effectively occur under highly dilute conditions. Next, intramolecularclick ring closure of star-linear PS-N3 was conducted under highly dilute conditions, using propargyl ether as thedifunctional linker and CuBr/PMDETA as the catalyst, affording quatrefoil-shaped star-cyclic PS. Gel permeationchromatography (GPC), 1H NMR, and FT-IR analysis confirmed the complete consumption of azide moieties instar-linear PS-N3 and that the coupling reaction proceeded via the intramolecular manner. Differential scanningcalorimetry (DSC) results revealed that star-cyclic PS possesses higher glass transition temperature (Tg) than thatof star-linear PS, possibly due to the ring topology of PS arms in the former.
The synthesis of polymers with varying chain topologies hasalways been the focus of polymer chemistry field due to thatchain architectures play an important role in determiningmacromolecular properties and functions in bulk and solutionstates.1-3 In the past decade, a variety of polymers withintriguing topologies, such as cyclic,4-6 linear-cyclic,7,8 linear-dendritic,9,10 dendronized,11-13 Y-shaped,14,15 H-shaped,16-18
ABC miktoarm star,18-21 hyperbranched,22-28 and dendriticpolymers29-32 have been prepared, partially due to the boomof controlled radical polymerization techniques and new con-cepts (click reaction, Diels-Alder reaction) borrowed frommodern organic chemistry.
Macrocyclic polymers represent the simplest nonlinear-shapedchain architecture consisting of only one type of monomerrepeating units. Recent developments in this area focused onthe fabrication of nonlinear polymers embedding with cyclicmotifs. Based on their previous experiences in preparing cyclicpolymers, Deffieux et al. prepared tadpole-shaped linear-cyclic,7 eight-shaped bicyclic,33 and macrotricyclic polymers34
by living anionic or cationic polymerization techniques. Tezukaet al.35,36 synthesized bicyclic and tricyclic polymers, as wellas monocyclic polymers covalently attached with single, double,and triple linear tails at predetermined positions via electrostaticself-assembly between terminally ionized linear precursors andmultifunctional coupling agent bearing opposite charges, andthe subsequent covalent fixation.37
It is worthy of noting that in the above examples, linearprecursors were typically synthesized via living anionic orcationic polymerizations. Though structurally well-defined intheir cases, the exploration of more convenient and mildsynthetic conditions is still desirable. In this context, theapplication of controlled radical polymerizations, such asnitroxide-mediated radical polymerization (NMP), atom transferradical polymerization (ATRP), and reversible addition-fragmen-tation chain transfer (RAFT) polymerization, as well as theconcept of click chemistry can be quite helpful. Grayson andco-workers4,5 prepared R-alkynyl--azido polystyrene (PS) byATRP, and macrocyclic PS can be obtained with high efficiencyby an intramolecular click ring closure reaction. Winnik et al.38
and our research group39,40 independently synthesized macro-cyclic poly(N-isopropylacrylamide) (PNIPAM) by the combina-tion of click reaction and RAFT or ATRP techniques. Recently,Pan et al.8 synthesized tadpole-shaped polymers consistingof linear PNIPAM and cyclic PS by coupling RAFT and clickreactions. They also successfully synthesized bicyclic polymersconsisting of PS and poly(-caprolactone) rings by couplingATRP, click, and ring-opening polymerization (ROP) tech-niques.41
To the best of our knowledge, the synthesis of star polymerswith macrocyclic arms has not been reported yet. Herein wereport a proof-of-concept example of the synthesis of quatrefoil-shaped star-cyclic polystyrene, star-cyclic PS, containing poly-hedral oligomeric silsesquioxane (POSS) core via the combi-nation of ATRP and click reactions (Schemes 1 and 2). 8-armstar-linear PS (star-linear PS-N3) bearing eight terminal azidefunctionalities was prepared by ATRP of styrene using POSS-* To whom correspondence should be addressed. E-mail: email@example.com.
2903Macromolecules 2009, 42, 2903-2910
10.1021/ma802585k CCC: $40.75 2009 American Chemical SocietyPublished on Web 03/31/2009
based octafunctional initiator, followed by the subsequentazidation reaction. Under click conditions, difunctional linkerpropargyl ether was slowly added via a syringe pump into theextremely dilute solution of star-linear PS-N3, leading to highefficiency preparation of quatrefoil-shaped star-cyclic PS bearingan inorganic POSS core.
Materials. Styrene (St, 99.5%, Beijing Chemical Factory) wassuccessively washed with aqueous NaOH (5.0 wt %) and water,then distilled over CaH2 at reduced pressure. CH2Cl2, anisole, andtriethylamine (TEA) were distilled over CaH2. Sodium azide(NaN3), copper(I) bromide (CuBr, 98%), N,N,N,N ,N -pentam-ethyldiethylenetriamine (PMDETA, 99%), propargyl alcohol, pro-pargyl ether, dimethyl 2,6-dibromoheptanedioate, and 2-bromoisobu-tyryl bromide were purchased from Aldrich and used as received.Merrifield resin was purchased from GL Biochem (Shanghai) Ltd.and used as received. Hydrofluoric acid (HF), 3-chloropropyltri-methoxysilane, and all other chemicals were purchased fromSinopharm Chemical Reagent Co. and used as received. Azido-functionalized Merrifield resin was prepared according to literature
Sample Preparation. Synthetic schemes employed for thepreparation of star-linear PS-N3 and star-cyclic PS were shown inSchemes 1 and 2.
Synthesis of Octafunctional POSS-(Cl)8. According to literatureprocedures,44 a mixture of methanol (1.8 L), 3-chloropropyltri-methoxysilane (79.5 g, 0.4 mol), and concentrated HCl (90 mL)was allowed to stir at room temperature for 5 weeks. POSS-(Cl)8was obtained as a white powder after suction filtration and washingwith deionized water (14.5 g, yield: 28%). 1H NMR (CDCl3, ,ppm, TMS): 0.74-0.88 (2H, Si-CH2-), 1.80-1.96 (2H,Si-CH2CH2-), 3.49-3.62 (2H, Si-CH2CH2CH2Cl). 13C NMR(CDCl3, , ppm): 9.4 (Si-CH2-), 26.3 (Si-CH2CH2-), 47.1(Si-CH2CH2CH2Cl). 29Si NMR (CDCl3, , ppm): -67.1 (Si-CH2-).
Synthesis of POSS-(N3)8. POSS-(N3)8 was prepared via azidationof POSS-(Cl)8. A typical procedure was as follows. Into a 100 mLround-bottom flask, NaN3 (6.5 g, 0.1 mol), POSS-(Cl)8 (3.0 g, 2.9mmol), and DMF (50 mL) were added. The flask was thenimmersed into an oil bath thermostated at 120 C. After stirringfor 2 days, the solvents were removed at reduced pressure. The
Scheme 1. Schematic Illustration for the Preparation of Octa(3-azidopropyl)polyhedral Oligomeric Silsesquioxane, POSS-(N3)8,POSS-Based Octafunctional ATRP Initiator, POSS-(Br)8, and POSS-Based 8-Arm Star Polystyrene, star-linear PS
Scheme 2. Schematic Illustration for the Synthesis of POSS-Based Quatrefoil-Shaped star-cyclic PS from 8-Arm star-linear PS-N3 viaIntramolecular Click Ring Closure with Propargyl Ether under Extremely Dilute Conditions
2904 Wang et al. Macromolecules, Vol. 42, No. 8, 2009
residues were dissolved in THF and passed through a neutralalumina column to remove residual sodium salts. A colorlessviscous liquid was obtained (2.5 g, yield: 79%) after drying in avacuum oven overnight at room temperature, and it is safe to storePOSS-(N3)8 in a desiccator at room temperature. 1H NMR (CDCl3,, ppm, TMS): 0.61-0.84 (2H, Si-CH2-), 1.54-1.83 (2H,Si-CH2CH2-), 3.24-3.47 (2H, Si-CH2CH2CH2N3). 13C NMR(CDCl3, , ppm): 9.8 (Si-CH2-), 22.8 (Si-CH2CH2-), 53.6(Si-CH2CH2CH2N3). 29Si NMR (CDCl3, , ppm): -69.1 (Si-CH2-).
Preparation of Propargyl 2-Bromoisobutyrate. Propargyl 2-bro-moisobutyrate was prepared by the esterification reaction ofpropargyl alcohol with 2-bromoisobutyryl bromide. In a typicalexample, propargyl alcohol (11.6 mL, 0.2 mol), triethylamine (27.8mL, 0.2 mol), and 100 mL of CH2Cl2 were added into a 250 mLthree-neck round-bottom flask. The mixture was cooled to 0 Cand 2-bromoisobutyryl bromide (24.7 mL, 0.2 mol) was addeddropwise over 2 h. The reaction mixture was stirred overnight atroom temperature. After removing insoluble salts by suctionfiltration, the filtrate was further purified by passing through a silicagel column using CH2Cl2 as the eluent. After removing all thesolvents by a rotary evaporator, the obtained residues were distilledunder reduced pressure, yielding a colorless liquid (30.8 g, yield:75%). 1H NMR (CDCl3, , ppm, TMS): 4.7 (2H, -CH2O), 2.5(1H, CHtC-), and 1.9 (6H, -C(CH3